#------------------------------------------------------------------------------
#$Date: 2016-02-14 06:40:26 +0200 (Sun, 14 Feb 2016) $
#$Revision: 176432 $
#$URL: svn://www.crystallography.net/cod/cif/7/01/99/7019969.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7019969
loop_
_publ_author_name
'Kan, Wei-Qiu'
'Yang, Jin'
'Liu, Ying-Ying'
'Ma, Jian-Fang'
_publ_section_title
;
 Inorganic-organic hybrid compounds based on octamolybdates and
 multidentate N-donor ligand: syntheses, structures, photoluminescence and
 photocatalysis.
;
_journal_issue                   36
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              11062
_journal_page_last               11073
_journal_paper_doi               10.1039/c2dt30755c
_journal_volume                  41
_journal_year                    2012
_chemical_formula_moiety         'C30 H30 Mo8 N16 O28 Zn'
_chemical_formula_sum            'C30 H30 Mo8 N16 O28 Zn'
_chemical_formula_weight         1895.59
_chemical_name_systematic
;
?
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                96.036(5)
_cell_angle_beta                 93.633(5)
_cell_angle_gamma                95.758(5)
_cell_formula_units_Z            1
_cell_length_a                   7.274(5)
_cell_length_b                   10.523(5)
_cell_length_c                   16.408(5)
_cell_measurement_reflns_used    3917
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      29.1999
_cell_measurement_theta_min      2.9942
_cell_volume                     1239.2(11)
_computing_cell_refinement       CrysAlis
_computing_data_collection       'CrysAlis (Oxford Diffraction, 2006)'
_computing_data_reduction        CrysAlis
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXL-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 10.0
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  'Oxford Diffraction Gemini R Ultra'
_diffrn_measurement_method       'ω scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71069
_diffrn_reflns_av_R_equivalents  0.0284
_diffrn_reflns_av_sigmaI/netI    0.0504
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            7907
_diffrn_reflns_theta_full        25.35
_diffrn_reflns_theta_max         25.35
_diffrn_reflns_theta_min         3.00
_exptl_absorpt_coefficient_mu    2.538
_exptl_absorpt_correction_T_max  0.6442
_exptl_absorpt_correction_T_min  0.5811
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlis (Oxford Diffraction, 2006)
;
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    2.540
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             912
_exptl_crystal_size_max          0.24
_exptl_crystal_size_mid          0.22
_exptl_crystal_size_min          0.19
_refine_diff_density_max         0.541
_refine_diff_density_min         -0.590
_refine_diff_density_rms         0.124
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.025
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     376
_refine_ls_number_reflns         4516
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.025
_refine_ls_R_factor_all          0.0395
_refine_ls_R_factor_gt           0.0300
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0242P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0622
_refine_ls_wR_factor_ref         0.0677
_reflns_number_gt                3837
_reflns_number_total             4516
_reflns_threshold_expression     >2σ(I)
_cod_data_source_file            c2dt30755c.txt
_cod_data_source_block           compound-4
_cod_original_sg_symbol_Hall     '-p 1'
_cod_original_sg_symbol_H-M      p-1
_cod_database_code               7019969
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Zn1 Zn 0.0000 -0.5000 0.5000 0.02486(19) Uani 1 2 d S
Mo1 Mo 0.34677(5) -0.33724(4) 0.38965(2) 0.01789(11) Uani 1 1 d .
Mo2 Mo 0.36393(5) -0.26260(4) 0.58584(2) 0.01756(11) Uani 1 1 d .
Mo3 Mo 0.27541(5) -0.03170(4) 0.45480(2) 0.01504(10) Uani 1 1 d .
Mo4 Mo 0.62089(5) -0.02974(4) 0.33344(2) 0.01944(11) Uani 1 1 d .
C1 C 0.1690(7) -0.2283(5) 0.2291(3) 0.0333(12) Uani 1 1 d .
H1 H 0.2794 -0.1758 0.2282 0.040 Uiso 1 1 calc R
C2 C -0.0325(6) -0.3600(5) 0.2679(3) 0.0239(11) Uani 1 1 d .
H2 H -0.0979 -0.4179 0.2974 0.029 Uiso 1 1 calc R
C3 C -0.2785(7) -0.3446(5) 0.1549(3) 0.0280(12) Uani 1 1 d .
H3A H -0.3517 -0.4127 0.1776 0.034 Uiso 1 1 calc R
H3B H -0.3403 -0.2672 0.1626 0.034 Uiso 1 1 calc R
C4 C -0.2123(7) -0.3499(5) -0.0527(3) 0.0265(11) Uani 1 1 d .
C5 C -0.1674(7) -0.2847(5) -0.1258(3) 0.0254(11) Uani 1 1 d .
C6 C -0.1622(7) -0.3563(5) -0.2012(3) 0.0310(12) Uani 1 1 d .
H6 H -0.1909 -0.4450 -0.2070 0.037 Uiso 1 1 calc R
C7 C -0.1135(7) -0.2937(6) -0.2676(3) 0.0366(13) Uani 1 1 d .
H7 H -0.1070 -0.3401 -0.3186 0.044 Uiso 1 1 calc R
C8 C -0.1274(8) -0.1530(5) -0.1195(3) 0.0366(13) Uani 1 1 d .
H8 H -0.1319 -0.1035 -0.0694 0.044 Uiso 1 1 calc R
C9 C -0.0811(8) -0.0960(6) -0.1873(4) 0.0444(15) Uani 1 1 d .
H9 H -0.0530 -0.0074 -0.1838 0.053 Uiso 1 1 calc R
C10 C -0.2604(6) -0.4968(5) 0.0234(3) 0.0258(11) Uani 1 1 d .
C11 C -0.2920(7) -0.6246(5) 0.0524(3) 0.0291(12) Uani 1 1 d .
C12 C -0.2924(8) -0.7332(6) -0.0026(3) 0.0399(14) Uani 1 1 d .
H12 H -0.2702 -0.7264 -0.0572 0.048 Uiso 1 1 calc R
C13 C -0.3259(9) -0.8506(6) 0.0247(4) 0.0513(17) Uani 1 1 d .
H13 H -0.3254 -0.9252 -0.0111 0.062 Uiso 1 1 calc R
C14 C -0.3567(8) -0.7469(7) 0.1548(3) 0.0482(17) Uani 1 1 d .
H14 H -0.3801 -0.7529 0.2094 0.058 Uiso 1 1 calc R
C15 C -0.3600(9) -0.8578(6) 0.1043(4) 0.0516(17) Uani 1 1 d .
H15 H -0.3851 -0.9370 0.1239 0.062 Uiso 1 1 calc R
N1 N 0.1361(5) -0.3028(4) 0.2896(2) 0.0226(9) Uani 1 1 d .
N2 N 0.0352(6) -0.2354(4) 0.1722(2) 0.0320(10) Uani 1 1 d .
N3 N -0.0940(5) -0.3223(4) 0.1976(2) 0.0216(9) Uani 1 1 d .
N4 N -0.2637(5) -0.3805(4) 0.0677(2) 0.0254(9) Uani 1 1 d .
N5 N -0.2315(5) -0.2851(4) 0.0187(2) 0.0280(10) Uani 1 1 d .
N6 N -0.2299(6) -0.4799(4) -0.0535(2) 0.0281(10) Uani 1 1 d .
N7 N -0.0766(6) -0.1689(5) -0.2585(3) 0.0402(12) Uani 1 1 d .
H7A H -0.0478 -0.1316 -0.3009 0.048 Uiso 1 1 calc R
N8 N -0.3220(7) -0.6292(5) 0.1315(2) 0.0401(12) Uani 1 1 d .
O1 O 0.1744(4) -0.4583(3) 0.40573(18) 0.0243(7) Uani 1 1 d .
O2 O 0.4788(4) -0.4049(3) 0.31924(18) 0.0303(8) Uani 1 1 d .
O3 O 0.4913(4) -0.3270(3) 0.48845(17) 0.0200(7) Uani 1 1 d .
O4 O 0.1993(4) -0.3947(3) 0.58451(17) 0.0238(7) Uani 1 1 d .
O5 O 0.5320(4) -0.2858(3) 0.65704(18) 0.0290(8) Uani 1 1 d .
O6 O 0.2008(4) -0.2023(3) 0.47332(16) 0.0163(6) Uani 1 1 d .
O7 O 0.2126(4) 0.0590(3) 0.54128(17) 0.0216(7) Uani 1 1 d .
O8 O 0.5029(4) 0.0761(3) 0.43889(16) 0.0158(6) Uani 1 1 d .
O9 O 0.1320(4) 0.0020(3) 0.37584(17) 0.0243(7) Uani 1 1 d .
O10 O 0.7644(4) 0.1378(3) 0.35416(17) 0.0204(7) Uani 1 1 d .
O11 O 0.4812(5) 0.0037(3) 0.25254(18) 0.0339(8) Uani 1 1 d .
O12 O 0.7737(5) -0.1219(4) 0.2895(2) 0.0382(9) Uani 1 1 d .
O13 O 0.4388(4) -0.1514(3) 0.37397(16) 0.0188(7) Uani 1 1 d .
O1W O 0.1307(5) -0.6624(4) 0.5095(2) 0.0497(11) Uani 1 1 d .
H1A H 0.2463 -0.6657 0.5154 0.075 Uiso 1 1 d R
H1B H 0.0620 -0.7289 0.5178 0.075 Uiso 1 1 d R
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1W Zn1 O1W 180.0(2) . 2_546
O1W Zn1 O4 89.69(15) . 2_546
O1W Zn1 O4 90.31(15) 2_546 2_546
O1W Zn1 O4 90.31(15) . .
O1W Zn1 O4 89.69(15) 2_546 .
O4 Zn1 O4 180.00(13) 2_546 .
O1W Zn1 O1 87.52(13) . .
O1W Zn1 O1 92.48(13) 2_546 .
O4 Zn1 O1 91.58(12) 2_546 .
O4 Zn1 O1 88.42(12) . .
O1W Zn1 O1 92.48(13) . 2_546
O1W Zn1 O1 87.52(13) 2_546 2_546
O4 Zn1 O1 88.42(12) 2_546 2_546
O4 Zn1 O1 91.58(12) . 2_546
O1 Zn1 O1 180.000(1) . 2_546
O2 Mo1 O1 105.91(16) . .
O2 Mo1 O3 103.98(15) . .
O1 Mo1 O3 99.80(14) . .
O2 Mo1 O13 95.11(14) . .
O1 Mo1 O13 152.78(13) . .
O3 Mo1 O13 91.47(13) . .
O2 Mo1 N1 91.04(15) . .
O1 Mo1 N1 82.12(15) . .
O3 Mo1 N1 163.54(13) . .
O13 Mo1 N1 80.37(13) . .
O2 Mo1 O6 166.11(14) . .
O1 Mo1 O6 87.12(13) . .
O3 Mo1 O6 77.87(11) . .
O13 Mo1 O6 71.03(11) . .
N1 Mo1 O6 85.94(12) . .
O5 Mo2 O4 104.75(16) . .
O5 Mo2 O10 101.41(14) . 2_656
O4 Mo2 O10 98.32(14) . 2_656
O5 Mo2 O3 96.23(14) . .
O4 Mo2 O3 97.31(13) . .
O10 Mo2 O3 152.54(12) 2_656 .
O5 Mo2 O8 94.30(14) . 2_656
O4 Mo2 O8 160.75(12) . 2_656
O10 Mo2 O8 74.79(12) 2_656 2_656
O3 Mo2 O8 83.11(12) . 2_656
O5 Mo2 O6 164.48(13) . .
O4 Mo2 O6 88.86(12) . .
O10 Mo2 O6 83.59(11) 2_656 .
O3 Mo2 O6 74.29(11) . .
O8 Mo2 O6 72.66(11) 2_656 .
O5 Mo2 Mo4 88.93(12) . 2_656
O4 Mo2 Mo4 132.27(10) . 2_656
O10 Mo2 Mo4 33.99(9) 2_656 2_656
O3 Mo2 Mo4 126.93(9) . 2_656
O8 Mo2 Mo4 43.82(7) 2_656 2_656
O6 Mo2 Mo4 87.26(7) . 2_656
O9 Mo3 O7 105.19(14) . .
O9 Mo3 O6 106.56(14) . .
O7 Mo3 O6 103.60(13) . .
O9 Mo3 O8 101.13(14) . .
O7 Mo3 O8 97.59(13) . .
O6 Mo3 O8 138.92(12) . .
O9 Mo3 O13 93.88(13) . .
O7 Mo3 O13 160.29(13) . .
O6 Mo3 O13 75.00(11) . .
O8 Mo3 O13 73.39(11) . .
O9 Mo3 O8 175.97(12) . 2_656
O7 Mo3 O8 77.37(12) . 2_656
O6 Mo3 O8 75.57(11) . 2_656
O8 Mo3 O8 75.31(12) . 2_656
O13 Mo3 O8 83.32(10) . 2_656
O12 Mo4 O11 104.27(17) . .
O12 Mo4 O10 102.23(16) . .
O11 Mo4 O10 97.04(15) . .
O12 Mo4 O13 104.66(16) . .
O11 Mo4 O13 95.91(15) . .
O10 Mo4 O13 146.12(11) . .
O12 Mo4 O8 154.20(14) . .
O11 Mo4 O8 101.50(14) . .
O10 Mo4 O8 73.39(11) . .
O13 Mo4 O8 73.41(11) . .
O12 Mo4 O7 84.16(14) . 2_656
O11 Mo4 O7 171.56(13) . 2_656
O10 Mo4 O7 81.21(12) . 2_656
O13 Mo4 O7 81.42(12) . 2_656
O8 Mo4 O7 70.07(10) . 2_656
O12 Mo4 Mo2 135.41(13) . 2_656
O11 Mo4 Mo2 90.04(12) . 2_656
O10 Mo4 Mo2 33.39(8) . 2_656
O13 Mo4 Mo2 115.74(8) . 2_656
O8 Mo4 Mo2 42.94(8) . 2_656
O7 Mo4 Mo2 83.98(8) 2_656 2_656
N2 C1 N1 115.0(5) . .
N2 C1 H1 122.5 . .
N1 C1 H1 122.5 . .
N1 C2 N3 109.6(4) . .
N1 C2 H2 125.2 . .
N3 C2 H2 125.2 . .
N4 C3 N3 109.8(3) . .
N4 C3 H3A 109.7 . .
N3 C3 H3A 109.7 . .
N4 C3 H3B 109.7 . .
N3 C3 H3B 109.7 . .
H3A C3 H3B 108.2 . .
N5 C4 N6 115.2(4) . .
N5 C4 C5 122.0(5) . .
N6 C4 C5 122.8(4) . .
C8 C5 C6 119.3(4) . .
C8 C5 C4 120.7(4) . .
C6 C5 C4 120.0(5) . .
C7 C6 C5 118.8(5) . .
C7 C6 H6 120.6 . .
C5 C6 H6 120.6 . .
N7 C7 C6 119.6(5) . .
N7 C7 H7 120.2 . .
C6 C7 H7 120.2 . .
C9 C8 C5 119.4(5) . .
C9 C8 H8 120.3 . .
C5 C8 H8 120.3 . .
N7 C9 C8 119.2(6) . .
N7 C9 H9 120.4 . .
C8 C9 H9 120.4 . .
N6 C10 N4 109.3(4) . .
N6 C10 C11 123.2(4) . .
N4 C10 C11 127.4(4) . .
N8 C11 C12 122.9(5) . .
N8 C11 C10 117.7(4) . .
C12 C11 C10 119.4(4) . .
C13 C12 C11 118.7(5) . .
C13 C12 H12 120.6 . .
C11 C12 H12 120.6 . .
C15 C13 C12 119.4(6) . .
C15 C13 H13 120.3 . .
C12 C13 H13 120.3 . .
N8 C14 C15 124.4(5) . .
N8 C14 H14 117.8 . .
C15 C14 H14 117.8 . .
C13 C15 C14 118.5(6) . .
C13 C15 H15 120.7 . .
C14 C15 H15 120.7 . .
C2 N1 C1 103.2(4) . .
C2 N1 Mo1 130.8(3) . .
C1 N1 Mo1 125.4(3) . .
C1 N2 N3 102.5(4) . .
C2 N3 N2 109.8(4) . .
C2 N3 C3 130.0(4) . .
N2 N3 C3 119.4(4) . .
C10 N4 N5 109.8(3) . .
C10 N4 C3 131.6(4) . .
N5 N4 C3 118.3(4) . .
C4 N5 N4 102.3(4) . .
C10 N6 C4 103.3(4) . .
C7 N7 C9 123.6(5) . .
C7 N7 H7A 118.2 . .
C9 N7 H7A 118.2 . .
C11 N8 C14 115.9(5) . .
Mo1 O1 Zn1 136.97(17) . .
Mo1 O3 Mo2 113.59(14) . .
Mo2 O4 Zn1 137.14(16) . .
Mo3 O6 Mo1 109.04(12) . .
Mo3 O6 Mo2 112.20(13) . .
Mo1 O6 Mo2 89.73(10) . .
Mo3 O7 Mo4 114.71(14) . 2_656
Mo3 O8 Mo2 148.68(15) . 2_656
Mo3 O8 Mo4 104.17(13) . .
Mo2 O8 Mo4 93.24(10) 2_656 .
Mo3 O8 Mo3 104.69(12) . 2_656
Mo2 O8 Mo3 98.49(11) 2_656 2_656
Mo4 O8 Mo3 97.39(10) . 2_656
Mo2 O10 Mo4 112.62(14) 2_656 .
Mo4 O13 Mo1 149.48(15) . .
Mo4 O13 Mo3 104.94(14) . .
Mo1 O13 Mo3 104.80(12) . .
Zn1 O1W H1A 126.3 . .
Zn1 O1W H1B 115.8 . .
H1A O1W H1B 116.7 . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Zn1 O1W 2.052(3) .
Zn1 O1W 2.052(3) 2_546
Zn1 O4 2.086(3) 2_546
Zn1 O4 2.086(3) .
Zn1 O1 2.115(3) .
Zn1 O1 2.115(3) 2_546
Mo1 O2 1.694(3) .
Mo1 O1 1.749(3) .
Mo1 O3 1.863(3) .
Mo1 O13 2.050(3) .
Mo1 N1 2.256(4) .
Mo1 O6 2.259(3) .
Mo2 O5 1.691(3) .
Mo2 O4 1.739(3) .
Mo2 O10 1.912(3) 2_656
Mo2 O3 1.989(3) .
Mo2 O8 2.188(3) 2_656
Mo2 O6 2.310(3) .
Mo2 Mo4 3.2072(15) 2_656
Mo3 O9 1.701(3) .
Mo3 O7 1.737(3) .
Mo3 O6 1.884(3) .
Mo3 O8 1.958(3) .
Mo3 O13 2.215(3) .
Mo3 O8 2.414(3) 2_656
Mo4 O12 1.693(3) .
Mo4 O11 1.708(3) .
Mo4 O10 1.942(3) .
Mo4 O13 1.946(3) .
Mo4 O8 2.224(3) .
Mo4 O7 2.383(3) 2_656
Mo4 Mo2 3.2072(15) 2_656
C1 N2 1.297(6) .
C1 N1 1.347(6) .
C1 H1 0.9300 .
C2 N1 1.321(6) .
C2 N3 1.324(6) .
C2 H2 0.9300 .
C3 N4 1.455(5) .
C3 N3 1.459(6) .
C3 H3A 0.9700 .
C3 H3B 0.9700 .
C4 N5 1.314(6) .
C4 N6 1.360(6) .
C4 C5 1.482(6) .
C5 C8 1.379(7) .
C5 C6 1.384(6) .
C6 C7 1.378(7) .
C6 H6 0.9300 .
C7 N7 1.304(7) .
C7 H7 0.9300 .
C8 C9 1.363(7) .
C8 H8 0.9300 .
C9 N7 1.334(7) .
C9 H9 0.9300 .
C10 N6 1.321(5) .
C10 N4 1.359(6) .
C10 C11 1.475(7) .
C11 N8 1.334(6) .
C11 C12 1.380(7) .
C12 C13 1.362(8) .
C12 H12 0.9300 .
C13 C15 1.353(8) .
C13 H13 0.9300 .
C14 N8 1.339(7) .
C14 C15 1.356(9) .
C14 H14 0.9300 .
C15 H15 0.9300 .
N2 N3 1.361(6) .
N4 N5 1.361(5) .
N7 H7A 0.8600 .
O7 Mo4 2.383(3) 2_656
O8 Mo2 2.188(3) 2_656
O8 Mo3 2.414(3) 2_656
O10 Mo2 1.912(3) 2_656
O1W H1A 0.8447 .
O1W H1B 0.8471 .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
N5 C4 C5 C8 6.0(7) . .
N6 C4 C5 C8 -171.5(5) . .
N5 C4 C5 C6 -175.2(4) . .
N6 C4 C5 C6 7.3(7) . .
C8 C5 C6 C7 1.2(7) . .
C4 C5 C6 C7 -177.7(4) . .
C5 C6 C7 N7 -1.1(8) . .
C6 C5 C8 C9 -0.8(8) . .
C4 C5 C8 C9 178.0(5) . .
C5 C8 C9 N7 0.4(8) . .
N6 C10 C11 N8 -179.7(4) . .
N4 C10 C11 N8 -2.2(7) . .
N6 C10 C11 C12 -0.8(7) . .
N4 C10 C11 C12 176.8(5) . .
N8 C11 C12 C13 0.4(9) . .
C10 C11 C12 C13 -178.5(5) . .
C11 C12 C13 C15 0.8(9) . .
C12 C13 C15 C14 -1.0(10) . .
N8 C14 C15 C13 0.1(10) . .
N3 C2 N1 C1 0.8(5) . .
N3 C2 N1 Mo1 -170.0(3) . .
N2 C1 N1 C2 -0.1(6) . .
N2 C1 N1 Mo1 171.3(3) . .
O2 Mo1 N1 C2 107.4(4) . .
O1 Mo1 N1 C2 1.5(4) . .
O3 Mo1 N1 C2 -96.4(6) . .
O13 Mo1 N1 C2 -157.6(4) . .
O6 Mo1 N1 C2 -86.2(4) . .
O2 Mo1 N1 C1 -61.6(4) . .
O1 Mo1 N1 C1 -167.5(4) . .
O3 Mo1 N1 C1 94.6(6) . .
O13 Mo1 N1 C1 33.4(4) . .
O6 Mo1 N1 C1 104.8(4) . .
N1 C1 N2 N3 -0.6(6) . .
N1 C2 N3 N2 -1.3(5) . .
N1 C2 N3 C3 -170.8(4) . .
C1 N2 N3 C2 1.1(5) . .
C1 N2 N3 C3 171.9(4) . .
N4 C3 N3 C2 -135.7(5) . .
N4 C3 N3 N2 55.7(5) . .
N6 C10 N4 N5 -1.0(5) . .
C11 C10 N4 N5 -178.8(4) . .
N6 C10 N4 C3 -174.9(4) . .
C11 C10 N4 C3 7.3(8) . .
N3 C3 N4 C10 89.4(6) . .
N3 C3 N4 N5 -84.1(5) . .
N6 C4 N5 N4 0.0(5) . .
C5 C4 N5 N4 -177.7(4) . .
C10 N4 N5 C4 0.6(5) . .
C3 N4 N5 C4 175.4(4) . .
N4 C10 N6 C4 1.0(5) . .
C11 C10 N6 C4 178.9(4) . .
N5 C4 N6 C10 -0.6(5) . .
C5 C4 N6 C10 177.0(4) . .
C6 C7 N7 C9 0.7(8) . .
C8 C9 N7 C7 -0.4(8) . .
C12 C11 N8 C14 -1.2(8) . .
C10 C11 N8 C14 177.7(5) . .
C15 C14 N8 C11 1.0(9) . .
O2 Mo1 O1 Zn1 156.0(2) . .
O3 Mo1 O1 Zn1 48.3(3) . .
O13 Mo1 O1 Zn1 -64.8(4) . .
N1 Mo1 O1 Zn1 -115.1(3) . .
O6 Mo1 O1 Zn1 -28.8(2) . .
O1W Zn1 O1 Mo1 -117.0(3) . .
O1W Zn1 O1 Mo1 63.0(3) 2_546 .
O4 Zn1 O1 Mo1 153.4(3) 2_546 .
O4 Zn1 O1 Mo1 -26.6(3) . .
O2 Mo1 O3 Mo2 -175.58(17) . .
O1 Mo1 O3 Mo2 -66.33(18) . .
O13 Mo1 O3 Mo2 88.79(16) . .
N1 Mo1 O3 Mo2 29.0(6) . .
O6 Mo1 O3 Mo2 18.55(14) . .
O5 Mo2 O3 Mo1 174.11(18) . .
O4 Mo2 O3 Mo1 68.32(18) . .
O10 Mo2 O3 Mo1 -56.0(3) 2_656 .
O8 Mo2 O3 Mo1 -92.29(16) 2_656 .
O6 Mo2 O3 Mo1 -18.42(14) . .
Mo4 Mo2 O3 Mo1 -92.54(16) 2_656 .
O5 Mo2 O4 Zn1 -152.0(2) . .
O10 Mo2 O4 Zn1 103.8(2) 2_656 .
O3 Mo2 O4 Zn1 -53.5(2) . .
O8 Mo2 O4 Zn1 36.5(5) 2_656 .
O6 Mo2 O4 Zn1 20.5(2) . .
Mo4 Mo2 O4 Zn1 105.7(2) 2_656 .
O1W Zn1 O4 Mo2 119.0(3) . .
O1W Zn1 O4 Mo2 -61.0(3) 2_546 .
O1 Zn1 O4 Mo2 31.5(2) . .
O1 Zn1 O4 Mo2 -148.5(2) 2_546 .
O9 Mo3 O6 Mo1 86.83(15) . .
O7 Mo3 O6 Mo1 -162.50(13) . .
O8 Mo3 O6 Mo1 -43.5(2) . .
O13 Mo3 O6 Mo1 -2.79(11) . .
O8 Mo3 O6 Mo1 -89.62(13) 2_656 .
O9 Mo3 O6 Mo2 -175.39(13) . .
O7 Mo3 O6 Mo2 -64.71(16) . .
O8 Mo3 O6 Mo2 54.3(2) . .
O13 Mo3 O6 Mo2 94.99(14) . .
O8 Mo3 O6 Mo2 8.16(10) 2_656 .
O2 Mo1 O6 Mo3 -0.3(6) . .
O1 Mo1 O6 Mo3 -160.41(15) . .
O3 Mo1 O6 Mo3 98.92(16) . .
O13 Mo1 O6 Mo3 3.08(12) . .
N1 Mo1 O6 Mo3 -78.12(16) . .
O2 Mo1 O6 Mo2 -113.8(5) . .
O1 Mo1 O6 Mo2 86.13(13) . .
O3 Mo1 O6 Mo2 -14.54(11) . .
O13 Mo1 O6 Mo2 -110.38(12) . .
N1 Mo1 O6 Mo2 168.42(13) . .
O5 Mo2 O6 Mo3 -43.0(5) . .
O4 Mo2 O6 Mo3 165.39(15) . .
O10 Mo2 O6 Mo3 66.88(15) 2_656 .
O3 Mo2 O6 Mo3 -96.70(15) . .
O8 Mo2 O6 Mo3 -9.15(11) 2_656 .
Mo4 Mo2 O6 Mo3 32.97(11) 2_656 .
O5 Mo2 O6 Mo1 67.5(5) . .
O4 Mo2 O6 Mo1 -84.10(13) . .
O10 Mo2 O6 Mo1 177.39(12) 2_656 .
O3 Mo2 O6 Mo1 13.81(11) . .
O8 Mo2 O6 Mo1 101.36(11) 2_656 .
Mo4 Mo2 O6 Mo1 143.48(8) 2_656 .
O9 Mo3 O7 Mo4 177.75(15) . 2_656
O6 Mo3 O7 Mo4 66.07(17) . 2_656
O8 Mo3 O7 Mo4 -78.48(16) . 2_656
O13 Mo3 O7 Mo4 -17.4(5) . 2_656
O8 Mo3 O7 Mo4 -5.46(13) 2_656 2_656
O9 Mo3 O8 Mo2 45.5(3) . 2_656
O7 Mo3 O8 Mo2 -61.7(3) . 2_656
O6 Mo3 O8 Mo2 177.4(2) . 2_656
O13 Mo3 O8 Mo2 136.3(3) . 2_656
O8 Mo3 O8 Mo2 -136.4(3) 2_656 2_656
O9 Mo3 O8 Mo4 -76.32(14) . .
O7 Mo3 O8 Mo4 176.49(13) . .
O6 Mo3 O8 Mo4 55.6(2) . .
O13 Mo3 O8 Mo4 14.44(10) . .
O8 Mo3 O8 Mo4 101.74(14) 2_656 .
O9 Mo3 O8 Mo3 -178.05(12) . 2_656
O7 Mo3 O8 Mo3 74.76(13) . 2_656
O6 Mo3 O8 Mo3 -46.2(2) . 2_656
O13 Mo3 O8 Mo3 -87.29(12) . 2_656
O8 Mo3 O8 Mo3 0.0 2_656 2_656
O12 Mo4 O8 Mo3 -106.0(3) . .
O11 Mo4 O8 Mo3 76.32(17) . .
O10 Mo4 O8 Mo3 170.32(15) . .
O13 Mo4 O8 Mo3 -16.49(12) . .
O7 Mo4 O8 Mo3 -103.20(14) 2_656 .
Mo2 Mo4 O8 Mo3 153.75(17) 2_656 .
O12 Mo4 O8 Mo2 100.3(3) . 2_656
O11 Mo4 O8 Mo2 -77.43(15) . 2_656
O10 Mo4 O8 Mo2 16.58(11) . 2_656
O13 Mo4 O8 Mo2 -170.24(13) . 2_656
O7 Mo4 O8 Mo2 103.05(12) 2_656 2_656
O12 Mo4 O8 Mo3 1.3(4) . 2_656
O11 Mo4 O8 Mo3 -176.44(13) . 2_656
O10 Mo4 O8 Mo3 -82.43(13) . 2_656
O13 Mo4 O8 Mo3 90.75(13) . 2_656
O7 Mo4 O8 Mo3 4.05(10) 2_656 2_656
Mo2 Mo4 O8 Mo3 -99.00(12) 2_656 2_656
O12 Mo4 O10 Mo2 -174.41(16) . 2_656
O11 Mo4 O10 Mo2 79.28(17) . 2_656
O13 Mo4 O10 Mo2 -32.5(3) . 2_656
O8 Mo4 O10 Mo2 -20.68(13) . 2_656
O7 Mo4 O10 Mo2 -92.39(15) 2_656 2_656
O12 Mo4 O13 Mo1 1.2(3) . .
O11 Mo4 O13 Mo1 107.6(3) . .
O10 Mo4 O13 Mo1 -140.3(3) . .
O8 Mo4 O13 Mo1 -152.1(3) . .
O7 Mo4 O13 Mo1 -80.4(3) 2_656 .
Mo2 Mo4 O13 Mo1 -159.5(3) 2_656 .
O12 Mo4 O13 Mo3 167.86(15) . .
O11 Mo4 O13 Mo3 -85.69(16) . .
O10 Mo4 O13 Mo3 26.4(3) . .
O8 Mo4 O13 Mo3 14.59(10) . .
O7 Mo4 O13 Mo3 86.24(12) 2_656 .
Mo2 Mo4 O13 Mo3 7.22(14) 2_656 .
O2 Mo1 O13 Mo4 -16.7(3) . .
O1 Mo1 O13 Mo4 -157.5(3) . .
O3 Mo1 O13 Mo4 87.5(3) . .
N1 Mo1 O13 Mo4 -106.9(3) . .
O6 Mo1 O13 Mo4 164.1(3) . .
O2 Mo1 O13 Mo3 176.62(14) . .
O1 Mo1 O13 Mo3 35.8(3) . .
O3 Mo1 O13 Mo3 -79.20(13) . .
N1 Mo1 O13 Mo3 86.43(14) . .
O6 Mo1 O13 Mo3 -2.56(10) . .
O9 Mo3 O13 Mo4 83.84(16) . .
O7 Mo3 O13 Mo4 -81.5(4) . .
O6 Mo3 O13 Mo4 -170.04(16) . .
O8 Mo3 O13 Mo4 -16.63(12) . .
O8 Mo3 O13 Mo4 -93.24(13) 2_656 .
O9 Mo3 O13 Mo1 -103.10(15) . .
O7 Mo3 O13 Mo1 91.5(4) . .
O6 Mo3 O13 Mo1 3.01(12) . .
O8 Mo3 O13 Mo1 156.43(15) . .
O8 Mo3 O13 Mo1 79.81(13) 2_656 .
